metals Review Literature Review and Thermodynamic Modelling of Roasting Processes for Lithium Extraction from Spodumene Allen Yushark Fosu 1 , Ndue Kanari 1 , James Vaughan 2 and Alexandre Chagnes 1, * 1 2 * CNRS, GeoRessources, Université de Lorraine, 54000 Nancy, France; [email protected] (A.Y.F.); [email protected] (N.K.) School of Chemical Engineering, The University of Queensland, Brisbane, QLD 4072, Australia; [email protected] Correspondence: [email protected]; Tel.: +33(0)-372-744-544 Received: 24 August 2020; Accepted: 28 September 2020; Published: 30 September 2020 Abstract: This review adds to the public domain literature on the extraction of lithium from mineral ores. The focus is on the pyrometallurgical pre-treatment of spodumene. Information on the phase transformation from α to β, the heat treatment methods as well as the behavior of various compounds in the roasting processes are evaluated. Insight into the chemical thermodynamics of the baking process is evaluated using HSC Chemistry software up to 1200 ◦ C. It was observed that the alkaline, sulfation, chlorination (using Cl2 and CaCl2 ), carbonizing (to form Li2 CO3 ) and fluorination processes were feasible either throughout or at a point within the temperature range considered. Chlorination using KCl and carbonizing to form Li2 O are the processes found to be nonspontaneous throughout the temperatures considered. Keywords: spodumene; thermodynamics; lithium; roasting 1. Introduction Lithium is used in several industries as a component of products such as glass–ceramics, greases and casting-alloys. Over the last two decades, lithium’s use in batteries, particularly for making vehicles, has resulted in an increased need for lithium compounds. Global lithium demand has risen to about 60% in this time and a 20% yearly increase is expected over the next few decades [1,2]. Such a boom in lithium production is accompanied by a drastic increase of its price, which has tripled in a little more than three years (from 5000 US dollars per ton in 2014 to more than 15,000 US dollars per ton by the end of 2017) . The astronomical demand for the metal has caught the attention of metallurgists around the globe and has prompted the development of novel beneficiation approaches to meet this demand by focusing on extraction from mineral ores. Extracting lithium from ores has higher operating costs than conventional extraction from brine, however, the theory of supply and demand makes the processing economically prudent because of the increasing price of lithium. Spodumene is the main ore of interest due to its high lithium content (~8 wt.% as Li2 O in a pure mineral specimen) [4,5]. Table 1 shows the mineralogical composition of a typical spodumene ore sample with 2.14 wt.% Li2 O. The concentration of Li2 O in this ore indicates that it is low grade. Spodumene is a lithium aluminum silicate (Li2 O·Al2 O3 ·4SiO2 or LiAlSi2 O6 ) of the pyroxene group; it is found in close association with quartz, feldspar and micas . Its color may vary from purple, green, yellow, gray or white, depending on the presence and concentrations of sodium, manganese, iron, magnesium or titanium [7–9]. Spodumene is naturally present in the stable α-monoclinic (highly packed crystal structure) form with high grindability and hence the mineral is difficult to leach without pretreatment. It is made Metals 2020, 10, 1312; doi:10.3390/met10101312 www.mdpi.com/journal/metals Metals 2020, 10, 1312 2 of 17 amenable to lixiviation by calcination at 1000 ◦ C to the β-tetragonal form . During the thermal process, there is a dislocation of Al3+ in the α-spodumene leading to aβ-spodumene crystal structure with a comparably larger crystal volume. This increases the mobility of lithium atoms which then become easily accessible to aqueous lixiviant solutions [4,10,11]. The phase transformation has also been shown to improve comminution, as β-spodumene is relatively soft and flaky [9,10,12]. Recently, an intermediary hexagonal metastable γ-phase was discovered during calcination. This phase is predicted to influence the extraction of lithium. Therefore the sequence of the phase transformation is now understood to be α→γ→β [4,10,13]. Though interlocking gangue in spodumene can adversely affect downstream beneficiation processes, Salakjani et al.  as well as White and McVay  indicated that these impurities facilitate heat conduction and efficient transformation since spodumene itself exhibits low thermal conductivity. Table 1. The mineralogical composition of a typical spodumene ore sample. Mineral Cr2 O3 MgO MnO Li2 O SO3 Fe2 O3 K2 O Na2 O TiO2 P2 O5 SiO2 Al2 O3 CaO % 0.03 1.30 0.32 2.14 0.15 4.29 1.26 1.14 0.10 0.33 61.31 20.79 1.72 Prior to the hydrometallurgical treatment of the ore after calcination, the β-spodumene phase is baked or roasted with additional compounds which define the next processing route as acidic, alkaline or chlorination. This review focuses on the various methods of processing spodumene ore, providing theoretical insight from the thermodynamic point of view using the reaction equation and the equilibrium module of HSC Chemistry software version 5.1 (Outokumpu Research Oy, Pori, Finland). 2. Decrepitation of Spodumene Ore The amenability of spodumene to lixiviation is greatly enhanced by its transformation from the α-form to β-form at elevated temperature, however, a process for direct extraction of lithium from α-spodumene using the HF/H2 SO4 system was introduced by Guo et al. . The thermal behavior of spodumene has been studied extensively by a number of researchers [4,5,10,11,16] and it is worthy to note that the process is carried out below 1040 ◦ C which is the fusion temperature of spodumene . It has been established that the phase change of α-phase spodumene starts at 800 ◦ C and is completed by 1100 ◦ C, though there is a report of the phase transformation commencing above 634 ◦ C using microwave heating [5,10]. Peltosaari et al.  considered the effect of particle size to be insignificant with respect to the conversion rate of spodumene. Salakjani et al.  revealed that heating leads to volumetric expansion and makes the ore porous. The final β-spodumene consequently has a larger surface area which enhances subsequent chemical processing. They found that a greater extent of the β-spodumene formed corresponded to a higher surface area produced but a relatively low density. It is anticipated that the inversion of α-spodumene to γ-spodumene is exothermic and that the heat released helps to offset the heat requirement of the process, however, the phase change from α directly to β is endothermic [9,18]. Investigations by Moore et al.  indicate that the temperature and the heating method have negligible effect on the mass fraction of the phases transformed during the decrepitation process and that the quantities of inversion products are almost equal at the initial stage before the final conversion to the β-phase. Conversely, Salakjani et al.  explained that temperature and residence time are the major factors that determine the inversion of the phases in spodumene; the temperature requirement is subsequently influenced by the chemical composition and the feed particle size of the spodumene sample. The phase transformation process at the elevated temperature is known to be influenced by many factors including the heating method employed, the morphology of the sample after comminution and the quantity of gangue minerals present [4,10,11,16]. Recently, microwave heat treatment of spodumene has been studied extensively by several authors and compared with conventional methods [4,5,10,16,19]. Spodumene is passive to microwave Metals 2020, 10, 1312 3 of 17 irradiation so the heat treatment with this method is made possible by hybrid microwave heating with the aid of SiC [9,10]. It was found that β-phase spodumene absorbs significantly higher microwave energy than the α-phase spodumene, resulting in local sintering when the β-phase is reached . Treatment of spodumene using microwave irradiation is still under development and much additional research is required to overcome challenges such as local sintering that results in unequal heating, transparency of spodumene to microwave irradiation and other factors that generally affect the treatment of ores using microwave irradiation. Salakjani et al.  suggested that mechanical stirring and the addition of additives (which do not affect downstream processes) could be a remedy for the sintering and passive behavior of spodumene to microwave irradiation, respectively. The microwave heat treatment was found to have a fast transformation rate compared with conventional heating. The transformation of α-spodumene commenced and was almost complete at 110 and 170 s of microwave irradiation respectively , but it appears that an hour of heating in a muffle furnace is needed to achieve a 100% conversion to the β-phase . The operating temperature was, however, found to be invariant with regards to the heating methods. There appears to be an inconsistency in the inversion temperatures of these two investigations during the conventional approach. According to Salakjani et al. , no phase change was observed for temperatures below 950 ◦ C irrespective of the heating time. They observed the first γ and β-phases at 950 ◦ C for at least 30 min of residence time but Peltosaari et al.  observed the first γ-phase at 800 ◦ C. This inconsistency might be due to some factors such as the concentration of impurities, the amorphous nature created due to the mechanical treatment and even particle size to a lesser degree. A minimum of 5 min of conventional heating at 1100 ◦ C was observed by Salakjani et al.  to almost complete the conversion of α to β-spodumene while Peltosaari et al.  indicated that 100% conversion was achieved within 15 min. However, Salakjani et al.  observed some γ-phase present even after 1-h of residence time at 1100 ◦ C. Comparing the energy requirement for the microwave and the muffle furnace heating for the phase conversion process shows that the microwave approach requires a relatively low energy input for the transformation compared to the conventional method . The conversion to the β-phase requires 5 times less energy by using microwave heating than conventional furnace. The reason for the high energy requirement in the conventional process can be due to the fact that heating begins from the outside and moves to the inside of the sample by conduction (the furnace needs to heat up evenly before the sample undergoes heating) therefore, most of the energy is wasted while in the microwave process, heating starts from the inside of the sample and extends radially outside (the sample absorbs the microwave radiation directly for heating), leading to little or no loss of energy. In another paper , the comparison of the microwave and conventional heat treatment for acid roasting of β-spodumene showed that microwave heating resulted in higher lithium extraction than the muffle furnace with regards to key parameters like processing time, excess acid and energy requirement. Indeed, 10.4 MJ of energy was needed for the conventional process whereas only 15.4 kJ was required for the microwave for the same quantity of lithium extracted. Microwave irradiation again required shorter time (20 s) to achieve this goal while an hour was needed in the muffle furnace for the extraction. Particle size was found to have an important effect on the amount of lithium extracted by microwave heat. Finer particles have been confirmed to enhance maximum (93%) lithium extraction with as low as 15% excess acid requirement as compared to 80% excess acid, which is normally used in roasting. 3. Roasting of Spodumene Ore Roasting β-spodumene with appropriate reagents results in a chemoselective ion exchange reaction where lithium is exchanged for atoms of similar characteristics in the reagent used. This may be done after decrepitation where β-spodumene is roasted with chemicals, or may be performed in-situ during decrepitation. This leads to the formation of soluble lithium salt (such as LiCl, Li2 SO4 or LiOH). Various reagents have been employed for forming the lithium salt during roasting and rigorous investigations are ongoing for optimization. Unlike roasting, the decrepitation process appears to be nearly optimized and little can be done to further adjust parameters like the operation temperature Metals 2020, 10, x FOR PEER REVIEW 4 of 18 Metals 2020,investigations 10, 1312 rigorous 4 of 17 are ongoing for optimization. Unlike roasting, the decrepitation process appears to be nearly optimized and little can be done to further adjust parameters like the operation temperature and granulometry of the ore used . for Thethe reagent for the the roasting and granulometry of the comminuted orecomminuted . The reagent roastingused determines name determines the name of the process. Generally, at a given pH, reagents are selected based their of the process. Generally, at a given pH, reagents are selected based on their selectivity for the on metal of selectivity for the metal of interest, stability in the aqueous phase, environmental friendliness, cost interest, stability in the aqueous phase, environmental friendliness, cost and ease of regeneration after and ease of regeneration after dissolution. These reasons have resultedininsearch a series investigations in dissolution. These reasons have resulted in a series of investigations ofof suitable chemicals search of suitable chemicals that satisfy a majority of these criteria during lithium ore beneficiation. that satisfy a majority of these criteria during lithium ore beneficiation. There forfor roasting spodumene. The first acidisroasting, which There are are three threewell-known well-knownmethods methods roasting spodumene. Theisfirst acid roasting, involves baking the calcined spodumene product with an excess of concentrated sulphuric acid at a which involves baking the calcined spodumene product with an excess of concentrated sulphuric acid temperature of about 250 °C (for conventional heat treatment) or 320 °C (for microwave irradiation at a temperature of about 250 ◦ C (for conventional heat treatment) or 320 ◦ C (for microwave irradiation for 20 s) s) . . The The second second is is the the alkaline alkaline process process which which utilizes utilizes limestone limestone (CaCO (CaCO3)) or or lime lime (Ca(OH) (Ca(OH)2 for 20 3 2 or CaO) and lastly, the chloride route which uses various chlorinating reagents. There are other or CaO) and lastly, the chloride route which uses various chlorinating reagents. There are other new new approaches such as as the the carbonizing carbonizing (using (using Na Na2CO CO3 in the presence of CO2 and other additives) and approaches such 2 3 in the presence of CO2 and other additives) and fluorination (using NaF). Figure 1 shows the main high-temperature for spodumene fluorination (using NaF). Figure 1 shows the main high-temperature routes forroutes spodumene treatments treatments which are described below (sulfation, alkaline and chlorination processes processing which are described below (sulfation, alkaline and chlorination processes for processingfor spodumene). spodumene). Figure 1. The flow diagram of the major treatment processes for spodumene (chlorination, sulfation Figure 1. The flow diagram of the major treatment processes for spodumene (chlorination, sulfation and alkaline processes). and alkaline processes). 3.1. Sulfation Processing of Spodumene In this process, alkali metal sulfates, sulfates, sulfuric sulfuric acid acid or or SO SO33 gas in the presence of water and oxygen employedasasreagent reagent to produce soluble lithium sulfate be leached. water leached. This are employed (s)(s) to produce soluble lithium sulfate whichwhich can becan water This process process benefits high stability and solubility ofsulfate lithiuminsulfate in the aqueous phaseleaching. during benefits from thefrom high the stability and solubility of lithium the aqueous phase during leaching. The drawbacks are the difficulty in producing high purity lithium carbonate resulting The drawbacks are the difficulty in producing high purity lithium carbonate resulting fromfrom the the unselectivity of sulfate reagents towards other metals asNa, Al, Mg, Na, Mg, Fe and K. Aluminum unselectivity of sulfate reagents towards other metals suchsuch as Al, Fe and K. Aluminum and and iron impurities be significant that precipitating from the leachate iron impurities may may be significant such such that precipitating them them from the leachate carriescarries along along some some lithium, decreasing overall lithium recovery The presence of some alkali metals affects lithium, decreasing overall lithium recovery . . The presence of some alkali metals alsoalso affects the the purity of the final product since they leachedalongside alongsidelithium lithiumand andseparating separating them them becomes purity of the final product since they areare leached aqueous solution. solution. complicated due to their similar chemistry to lithium in aqueous The sulfation process consumes a large amount of reagent which affects the economic viability of the process [20,21]. Sulfates of potassium, ammonium and sodium have been successfully used for the Metals 2020, 10, 1312 5 of 17 extraction of lithium from several lithium bearing minerals. Sulfate roasting of lepidolite followed by water leaching has been studied widely using Na2 SO4 /K2 SO4 /CaO, Na2 SO4 and FeSO4 at roasting temperatures of 880, 1000, 850 ◦ C respectively. The corresponding approximate extraction extents were 95, 99.5 and 90% extraction, respectively [21–24]. The sulfating behavior of zinnwaldite, petalite and montmorillonite have also been discussed elsewhere [21,25–27] using Na2 SO4 and H2 SO4 and yielding 90, 97.3 and 90% lithium extraction, respectively. In the case of spodumene, the transformation from the α to the β-phase is crucial before the application of sulphates as indicated above. Several authors have conducted systematic experimental studies to understand and optimize the amenability of sulfates to spodumene beneficiation [17,19,28–31]. The use of sulfuric acid is renowned and currently, the commercialized process for lithium extraction while the others are still undergoing research. In the acid process, the ore is roasted with sulfuric acid at a temperature of about 250 ◦ C. Investigations by Salakjani et al.,  indicate that one hour is optimal for conventional heating while only 20 s is needed with microwave roasting. It is essential that this process is operated below 337 ◦ C to prevent the evaporation of the acid . During this process, the H+ of the acid is chemoselectively exchanged with Li+ of spodumene as indicated in Equation (1) to form water soluble Li2 SO4(s) . The water-soluble part of the roasting process is water leached according to Equation (2), lime precipitation is conducted at 90 ◦ C for pH adjustment and removal of impurities from solution. Lithium carbonate is recovered by the addition of sodium carbonate solution to the extract as indicated by Equation (3): 2LiAlSi2 O6(s) + H2 SO4(l) → Li2 SO4(s) + 4SiO2(s) + Al2 O3(s) + H2 O(g) (1) Li2 SO4(s) → Li2 SO4(aq) (2) Li2 SO4(aq) + Na2 CO3(aq) → Li2 CO3(s) + Na2 SO4(aq) (3) It must be noted that the diffusion of the acid through the ore for the ion exchange is the rate determining step for the reaction. Unlike gaseous reagents, the viscous nature of the liquids (acid and lithium bisulphate produced around 170 ◦ C) slows their penetration through tiny pores and cracks, thereby slowing down the reaction . 3.2. Alkaline Process This process benefits from the economics and the nonaggressive nature of the salt used as a reagent compared to the acid process which requires the use of concentrated acid . It involves roasting the lithium bearing ore with lime or limestone within the temperature range of 100–205 ◦ C or 825–1050 ◦ C respectively. Roasting with limestone is specified by Equation (4) where water soluble Li2 O(s) is formed with calcium aluminosilicate and carbon dioxide. Li2 O(s) is water leached to produce aqueous LiOH [21,34], which is separated from residual solids by filtration. Instead of direct baking of spodumene with limestone to produce Li2 O(s) , limestone can initially be decomposed thermally to produce CaO (Equation (5)).The CaO that was produced is then roasted with spodumene in the presence of water to produce LiOH (Equation (6)). Li2 O·Al2 O3 ·4SiO2(s) + CaCO3(s) → Li2 O(s) + CaO·Al2 O3 ·4SiO2(s) + CO2(g) (4) CaCO3(s) → CaO(s) + CO2(g) (5) LiAlSi2 O6(s) + CaO(s) + H2 O(l) → LiOH(aq) + CaAl2 Si2 O8(s) (6) Metals 2020, 10, 1312 6 of 17 The lithium hydroxide that is produced can be converted to LiCl or LiCO3 by reaction with hydrochloric acid or carbon dioxide, respectively, if they are the final products desired. This process has been used by Jandova et al.  to recover 90% lithium from zinnwaldite waste. Some additives such as gypsum, lithium carbonate and sodium sulphate may be employed in the baking process to enhance lithium recovery; recording 96%, 96% and 90%, respectively [33,36,37]. The downside of this approach is the high energy requirement for the decomposition of limestone and dicalcium silicate. This may result in the evolution of unbearable heat which makes temperature control in the system difficult . 3.3. Chlorination Process The use of chlorine gas and chloride bearing salts in mineral beneficiation is the least considered process due to the toxicity of chlorine gas that may be generated alongside the products, and the high cost of corrosion resistant equipment needed for the process. However, there are several benefits of chlorine metallurgy in minerals processing. The main benefit is the high selectivity of chlorine and the comparatively lower operating temperature. The generated chlorides have low melting and boiling points and are easily separated from the wastes due to the vapor pressure difference [38–40]. In addition, the use of chlorine results in high recovery of metals, which makes it easy for treating low grade ores. Lastly, the process results in the generation of environmentally green waste. These advantages call for a closer look at chlorine for beneficiating lithium ores, however, it has attracted little attention and few literature articles have been written about it [41–46]. Peterson et al.  patented a blend of muriate of potash and sylvinite ore (sodium and potassium chloride) to recover lithium from its ores at 980–1100 ◦ C. The reaction of this invention is an exchange reaction between the alkali metals of the chlorides and the lithium of the ore, thereby forming soluble LiCl, which was further converted to lithium carbonate by reaction with sodium carbonate. About 97.5% of the lithium carbonate was recovered by this approach. Chlorination of lepidolite using sodium and calcium chloride at 880 ◦ C yielded 93% lithium recovery . Recently, the same approach was applied to recover the lithium value in spodumene using chlorine gas and calcium chloride, respectively; 900 ◦ C and 120 min were suggested as the optimal chlorination conditions, which resulted in 90% lithium extraction when calcium chloride was used [43,44]. 3.4. Other Processes to Spodumene Treatment Other less known processes for beneficiating lithium ores worthy of discussion are the carbonizing and fluorination processing. Lithium carbonate can be produced by carbonizing lithium bearing ore with sodium carbonate between 525 and 675 ◦ C in a solid–solid intimate reaction followed directly by leaching or hydrothermal decomposition treatment (between 90 and 225 ◦ C) prior to leaching . The reactions of the process (Equations (7) and (8)) must be carried out above the minimum temperatures suitable for the individual lithium bearing ore (1080, 850, 980 and 870 ◦ C respectively for petalite, lepidolite, eucryptite and spodumene). They indicated the need to carry out this roasting in the presence of alkali metal chlorides, alkali metal sulfate or carbon dioxide which act as a catalyst for the process. However, a specific preference for sodium and potassium chloride or sulfate was indicated. By this process, 75–97% of lithium contained in the ore could be leached for recovery. The inventors of this process  highlighted some advantages of this process which include the possibility of using Na2 CO3 as the only reactant to produce Li2 CO3 of high purity. They indicated that the reagent is ideally employed to decompose refractory ores into fragments to enhance leaching. The process is therefore expected to require serious purification steps since the decomposition may give rise to several impurities. Using it as a plant production of Li2 CO3 with good recovery and high purity without major purification is therefore a breakthrough. This approach is also said to have a short processing time and to be economically viable. This is because, the reagent is added to the cooling calcined spodumene midway during the process, for it reacts with the mineral, thereby reducing the time for processing and also utilizing the energy which would have gone wasted. Metals 2020, 10, 1312 7 of 17 2LiAlSi2 O6(s) + Na2 CO3(s) + 4H2 O(l) → Li2 CO3(s) + Na2 O.Al2 O3 .4SiO2 .H2 O(s) (7) Li2 CO3(s) + CO2(g) + H2 O(l) → 2LiHCO3(s) (8) Owing to this invention several other investigations have revolved around it for its optimization [48,49]. Chen et al.  employed pressurized roasting of spodumene concentrate with sodium carbonate in an autoclave, yielding 94% lithium carbonate production with 99.6% purity. Research by dos Santos et al.  using spodumene and sodium carbonate, promoted by sodium chloride, resulted in 70% lithium yield. The involvement of NaCl by dos Santos et al.  was to aid the extraction of the residual lithium bound at the interstitial positions of the ore. This reaction was conducted within 550–650 ◦ C for 120 min. The only fluorination roasting report available in literature was performed by Rosales et al. , though there are some hydrometallurgical processes of spodumene beneficiation using some fluorination agents [15,51]. In this approach, roasting of NaF with β-spodumene at 600 ◦ C spodumene: NaF from 1:1 to 1:2.5 and 4 h was investigated. 90 % maximum lithium recovery was achieved and it occurred at spodumene: NaF of 1:2 and 2 h of roasting. Equation (9) illustrates the reaction process: 2LiAlSi2 O6(s) + 2NaF(s) → 2LiF(s) + NaAlSi3 O8(s) + NaAlSiO4(s) The processes discussed with some relevant information are summarized in Table 2. (9) Metals 2020, 10, 1312 8 of 17 Table 2. Summary of literature for the recovery of lithium from spodumene using the major beneficiation processes. Experimental Conditions Process Roasting Reagent Sulfating Alkaline Chlorination Carbonizing Fluorination Temp./ Leaching ◦C Time/min. Time/hr Temp./ ◦C Product Recovery/% Reference Lixiviant Conc.·H2 SO4 200–300 30–60 - - H2 O Li2 SO4 85  Na2 SO4 + CaO - - 3 230 Na2 SO4 + CaO Li2 SO4 93.30  Na2 SO4 + NaOH 200–300 - 3 230 Na2 SO4 + NaOH Li2 SO4 90.70  (NH4 )2 SO4 150–370 - - - NH3 (aq) Li2 SO4 -  CaSO4 + CaCO3 1000–1150 120–180 - - H2 O Li2 SO4 85–90  * Conc. H2 SO4 250–300 - 1 - H2 O Li2 SO4 86  H2 O+O2 + SO3 350–425 10-40 - - H2 O Li2 SO4 97  CaO + H2 O 100–205 60 H2 O LiOH ~97  CaO + H2 O 1000–1230 100 H2 O LiOH 80  * KCl, NaCl 1000–1050 15–60 - 85 H2 O/HCl LiCl 85–97.50  Cl2 1100 150 - - - LiCl -  CaCl2 900 120 - 60 H2 O LiCl 90.2  CaCl2 800–1200 - - - Alcohol LiCl 9.5–98.5  + Na2 CO3 525–675 10–120 - - H2 O, NH4 (aq) Li2 CO3 75–97  Na2 CO3 150–250 10–120 – - H2 O Li2 CO3 ~94  Na2 CO3 + NaCl ~923 120 - - H2 O Li2 CO3 70  NaF 600 120 0.5 25 HF LiF 90  * roasting of spodumene done in the alpha phase. Metals 2020, 10, 1312 9 of 17 4. Chemical Thermodynamics of Spodumene Processing Insight into thermodynamics of the beneficiation approaches of spodumene are scarce in literature. This section looks at the thermodynamic modelling of the various approaches of lithium processing encountered in literature using the HSC Chemistry software version 5.1 reaction equation and equilibrium module. The standard Gibbs free energy changes as a function of temperature for the following reactions involved during spodumene roasting with various reagents (sulfating, alkaline, fluorinating, carbonizing and chlorinating agents, Equations (10)–(22) are found in Figure 2: 2LiAlSi2 O6 (B)(s) + CaCl2(s) → 2LiCl(s) + 2SiO2(s) + CaAl2 Si2 O8(s) (10) 2LiAlSi2 O6 (B)(s) + Cl2(g) → 2LiCl(s) + 4SiO2(s) + Al2 O3(s) + 0.5O2(g) (11) 2LiAlSi2 O6 (B)(s) + Na2 CO3(s) → Li2 O(s) + 2NaAlSi2 O6(s) + CO2(g) (12) 2LiAlSi2 O6 (B)(s) + Na2 CO3(s) → Li2 CO3(s) + 2NaAlSi2 O6(s) (13) LiAlSi2 O6 (B)(s) + NaF(s) → LiF(s) + 0.5NaAlSi3 O8(s) + 0.5NaAlSiO4(s) (14) 2LiAlSi2 O6 (B)(s) + K2 SO4(s) → Li2 SO4(s) + 2KAlSi2 O6(s) (15) 2LiAlSi2 O6 (B)(s) + Na2 SO4(s) → Li2 SO4(s) + 2NaAlSi2 O6(s) (16) 0.5LiAlSi2 O6 (B)(s) + CaO(s) → 0.5LiAlO2(s) + CaSiO3(s) (17) 2LiAlSi2 O6 (B)(s) + H2 SO4(aq) → Li2 SO4(s) + 4SiO2(s) + Al2 O3(s) + H2 O(g) (18) 2LiAlSi2 O6 (B)(s) + SO3(g) + 3H2 O(g) → Li2 SO4(s) + 4SiO2(s) + 2Al(OH)3(s) (19) LiAlSi2 O6 (B)(s) + KCl(s) → LiCl(s) + 2SiO2(s) + KAlO2(s) (20) 6LiAlSi2 O6 (B)(s) + Fe2 (SO4 )3(s) → 3Li2 SO4(s) + 3Al2 O3(s) + Fe2 O3(s) + 12SiO2(s) (21) 6LiAlSi2 O6 (B)(s) + Al2 (SO4 )3(s) → 3Li2 SO4(s) + 4Al2 O3(s) + 12SiO2(s) Metals 2020, 10, x FOR PEER REVIEW (22) 10 of 18 Figure 2. 2. The The standard standard Gibbs Gibbs energies energies for for roasting roasting of of spodumene spodumene for for processes processes encountered encountered in in the the Figure literature (reactions (reactions (10)–(22)) (10)–(22)) versus versus temperature temperature (data (data from fromthe theHSC HSCChemistry Chemistry5.1 5.1software). software). literature To gain a deeper understanding of the approaches outlined in literature, the HSC Chemistry 5.1 software equilibrium module was further employed to investigate the equilibrium amount of each process as a function of temperature. Figure 3 displays the equilibrium moles for the sulfating process using Na2SO4, K2SO4, H2SO4, SO3(g)/H2O(g), Fe2(SO4)3 and Al2(SO4)3 as reagents. As indicated earlier (Figure 2), Na2SO4 is feasible only below 400 ℃. It is only below this temperature that the equilibrium moles of the products (lithium sulfate and sodium aluminosilicate, NaAlSiO6) are higher than Metals 2020, 10, 1312 10 of 17 It is worth noting from Figure 2 that all the reagents used in literature for alkaline, sulfating, fluorination, chlorination (with the exception of KCl) and carbonizing to yield Li2 CO3 were spontaneous at a point or throughout the operating temperature for roasting spodumene. Chlorination with KCl and carbonization to produce Li2 O were the only processes which are not thermodynamically favorable throughout the temperature range. All reagents for sulfating roasting except K2 SO4 and the feasible carbonizing process showed a major variation of spontaneity with temperature while reagents for other processes did not. Sulfation and chlorination using Na2 SO4 , SO3 and Cl2 as well as the spontaneous carbonizing process benefit from feasibility only at low temperatures; they are not feasible at high temperatures. The observed spontaneity of CaCl2 chlorination parallels observations by Barbosa et al. . However, those observations are contrary to observations made by the same authors earlier, which indicated feasibility with Cl2 even at higher temperatures . The reason for this difference is not yet apparent. To gain a deeper understanding of the approaches outlined in literature, the HSC Chemistry 5.1 software equilibrium module was further employed to investigate the equilibrium amount of each process as a function of temperature. Figure 3 displays the equilibrium moles for the sulfating process using Na2 SO4 , K2 SO4 , H2 SO4 , SO3(g) /H2 O(g) , Fe2 (SO4 )3 and Al2 (SO4 )3 as reagents. As indicated earlier (Figure 2), Na2 SO4 is feasible only below 400 ◦ C. It is only below this temperature that the equilibrium moles of the products (lithium sulfate and sodium aluminosilicate, NaAlSiO6 ) are higher than spodumene (Figure 3a), confirming feasibility. It can be inferred that the highest amount of lithium sulfate can be obtained below 200 ◦ C above which it starts decreasing until 400 ◦ C, where the reaction ceases feasibilityAround 400 ◦ C and above, solid lithium sulfate begins to change into a liquid state due to the increasing temperature but the amount is relatively smaller in the system; resulting from the decreased feasibility of the reaction. Temperatures less than 400 ◦ C appear to be the best for Na2 SO4 /spodumene roasting, however, 1000 ◦ C was required to achieve 90.4% lithium extraction according to Luong et al.  for Na2 SO4 /lepidolite roasting for 30 min. Unlike Na2 SO4 , K2 SO4 drives the reaction to the right within the whole temperature range considered, forming lithium sulfate in the solid phase (Figure 3b), moles of lithium sulfate then are at levels higher than spodumene within the entire temperature range considered. There is a steady decrease in moles of solid lithium sulfate and a simultaneous increase of the liquid phase with increasing temperature. This is a result of the conversion of the solid into liquid as liquid is formed until around the melting point (859 ◦ C); where all the solid phase changes to liquid and remains constant. Thermodynamics of the sulfuric acid process predicts feasibility throughout the entire temperature range considered (Figure 2) with ∆Go becoming more negative with increasing temperature. The highest amount of soluble Li2 SO4 produced by modelling of this process occurs around 200 ◦ C. When the temperature is close to 300 ◦ C and beyond, there is a steady decrease in quantity. These observations are in line with observations by Salakjani et al.  whose maximum recovery occurred at 250 ◦ C, but a decrease in lithium recovery was observed at 300 ◦ C and beyond. This occurrence is as a result of the decomposition of sulfuric acid between 300 and 400 ◦ C (Figure 3c). However, the process remains spontaneous even after the decomposition of the acid because the products of the decomposition (SO3 and H2 O) from Equation (23) are capable of driving the reaction to the product in Equation (25) but with a limited amount of lithium sulfate production. SO3 breaks down further into SO2 and O2 (Equation (24)), which remain as spectator species. Precautionary measures are advised at this point due to the toxicity of SO2 produced. Thus above 400 ◦ C the sulfuric acid process has thermodynamic behavior similar to the sulfation process using SO3(g) /H2 O(g) invented by Archambault et al. . considered. This is confirmed by Figure 4 where soluble lithium hydroxide is formed as the useful product. Other products formed include silica, silicates and other aluminosilicate with traces of calcium hydroxide. The moles of lithium hydroxide in the solid phase decreases sharply with increasing temperature. This occurrence is attributed to the conversion of the solid into the liquid phase, confirmed by the sharp rise of the liquid phase with increasing temperature until around its Metals 2020, 10, 1312 11 of 17 melting point (462 °C), where there is a total transformation into the liquid phase (Figure 4). Equilibrium amount (kmol) Equilibrium amount (kmol) 1.0 NaAlSi2O6 0.6 Na2SO4 0.9 K2SO4 0.5 LiAlSi2O6(B) 0.8 Li2SO4 KAlSi2O6 0.7 0.4 0.6 0.5 KAlSiO4 Li2SO4 0.3 0.4 KAlSi3O8 0.2 0.3 Li2SO4(l) 0.2 N2(g) 0.1 0.0 0.1 0 SiO2 N2(g) LiAlSi2O6(B) Li2SO4(l) 200 400 600 800 1000 0.0 1200 0 200 400 600 800 1000 1200 Temperature (°C) Temperature (°C) Metals 2020, 10, x FOR PEER REVIEW 12 of 18 (a) (b) Equilibrium amount (kmol) 2.0 Equilibrium amount (kmol) 2.0 SiO2 H2O(g) SiO2(B) SO2(g) 1.5 SO2(g) H2SO4 1.5 SO3(g) SO3(g) O2(g) 1.0 1.0 H2O(g) H2O O2(g) 0.5 Al2O3 Li2SO4 0.5 Al2O3 Li2SO4 LiAlSi2O6(B) LiAlSi2O6(B) Li2SO4(l) Li2SO4(l) N2(g) 0.0 0 N2(g) 200 400 600 800 1000 0.0 1200 0 200 400 600 Temperature (°C) (c) 1000 1200 (d) Equilibrium amount (kmol) Equilibrium amount (kmol) 2.0 1.5 800 Temperature (°C) 2.0 SiO2(B) SiO2 1.5 SO2(g) SO2(g) 1.0 0.5 O2(g) Li2SO4 Al2SiO5 Al2O3 1.0 0.5 Fe2O3 O2(g) Li2SO4 Fe2(SO4)3 Al2(SO4)3 SO3(g) N2(g) 0.0 0 200 400 600 800 1000 Li2SO4(l) LiAlSi2O6(B) SO3(g) N2(g) Fe3O4 FeSiO3 LiAlO2 0.0 1200 0 200 400 600 800 1000 1200 Temperature (°C) Temperature (°C) (e) (f) Figure 3. Equilibrium amounts temperature forroasting sulfate of roasting of spodumene (a) Figure 3. Equilibrium amounts versusversus temperature for sulfate spodumene using (a) Nausing 2 SO4 , Na 2SO4, (b) K2SO4, (c) H2SO4, (d) SO3(g), (e) Fe2(SO4)3 and (f) Al2(SO4)3 (data from HSC Chemistry 5.1 (b) K 2 SO4 , (c) H2 SO4 , (d) SO3(g) , (e) Fe2 (SO4 )3 and (f) Al2 (SO4 )3 (data from HSC Chemistry 5.1 software). software). Solid lithium sulfate in the reaction medium melts above 800 ◦ C. The equilibrium amount of Equilibrium amount (kmol) lithium sulfate decreases after 2.0 the decomposition of the acid but the kinetics of the process is expected to be favored due to the production of the gaseous reactants which easily access reaction sites by diffusion compared to the percolation of sulfuric acid as a result of its viscosity. Around 900 ◦ C and H2O H2O(g) 1.5 above the sulfation process with sulfuric acid and SO3(g) /H2 O(g) ceases spontaneity, signified by a sharp increase in the amount of spodumene in Figure 3c,d. This observation is attributed to the sintering LiOH(l) 1.0 LiOH effect and the formation of lithium silicate, which has close resemblance to β-sopodumene [54,55]. SiO2 Ca3Si2O7 0.5 Al2SiO5 H2 SO4(aq) →Ca2Al2SiO7 SO3(g) + H2 O(g) (23) N2(g) LiAlSi2O6(B) 0.0 0 200 400 600 800 1000 1200 Temperature (°C) Figure 4. Equilibrium amounts versus temperature for alkaline roasting of spodumene using CaO Metals 2020, 10, 1312 12 of 17 Metals 2020, 10, x FOR PEER REVIEW 2SO3(g) → 2SO2(g) + O2(g) (24) 12 of 18 Li2 O.Al2 O3 .4SiO2(s) + SO3(g) + 4H2 O(g) → Li2 SO4(s) + Al2 O3 .4SiO2 .H2 O(s) Equilibrium amount (kmol) (25) Equilibrium amount (kmol) 2.0 2.0 Spodumene roastingSiO2 using Fe2 (SO4 )3 and Al2 (SO4 )3 have similar behavior H2O(g) SiO2(B) (Figure 3e,f), except for a constant production of Li2 SO4 in the caseSO2(g) of Fe2 (SO4 )3 , but its amount is higher only at temperatures SO2(g) H2SO4 SO3(g) 1.5 ◦ C for Al (SO 1.5 producing SO /SO at higher temperatures, below 500 2 SO3(g)4 )3 . Metal sulfates also break down, 3 2 O2(g) which may influence the roasting process. According to Luong et al. , Na2 SO4 like K2 SO4 has high H2O 1.0 thermal1.0stability, ergo they break down at higher temperatures, producing a small H2O(g) amount of SO3 /SO2 , O2(g) which apparently has no effect on the process. This is confirmed by the absence of these gases in their Al2O3 Al2O3 Li2SO4 Li2SO4 modelled the amount of the gases generated 0.5 process (Figure 3a,b). For iron and aluminum sulfates, 0.5 LiAlSi2O6(B) LiAlSi2O6(B) Li2SO4(l) during theN2(g)decomposition is large enough to influence theN2(g) process. From Figure Li2SO4(l) 3e,f, the sulfate of these metals is 200 observed to600decompose around 700 ◦ C, producing the gases but their effect is minimal 0.0 0.0 0 400 800 1000 1200 0 200 400 600 800 1000 1200 (°C) Temperature (°C) due to the in spodumene as compared toTemperature observation in lepidolite by Luong et al. , which may be sintering of spodumene above 800 ◦ C [54,55]. (c) (d) Calcium oxide was considered the reagent for alkaline roasting of spodumene. LiAlO2 is Equilibrium (kmol) 2 produced from the reaction Equilibrium predicted by amount HSC(kmol) as a product of the reaction (Equation (17)).amount Ca(OH) 2.0 2.0 SiO2 of Equation (26) reacts with LiAlO2 (Equation (27)), producing LiOH in the solid or liquid phase dependingSiO2(B) on the temperature. 1.5 1.5 CaO(s) SO2(g) + H2 O(g) → Ca(OH)2(s) 1.0 0.5 Li2SO4 Al2SiO5 Fe2(SO4)3 SO2(g) (26) O2(g) (27) Al2O3 1.0 O2(g) Li2SO4 2LiAlO2(s) 0.5 (s) + CaAl2 O4(s) Fe2O3 + Ca(OH)2(s) → 2LiOH Al2(SO4)3 Li2SO4(l) LiAlSi2O6(B) SO3(g) N2(g) It canN2(g)be found from FigureSO3(g) 2 that the range Fe3O4 process is feasible throughout the temperature LiAlO2 FeSiO3 0.0 0.0 0 200 is confirmed 400 600 1000 4 where 1200 0 200 hydroxide 400 600is formed 800 1000 the 1200 considered. This by800Figure soluble lithium as useful Temperature (°C) Temperature (°C) product. Other products formed include silica, silicates and other aluminosilicate with traces of calcium hydroxide. The moles of lithium hydroxide in the solid phase decreases sharply with increasing (e) (f) temperature. This occurrence is attributed to the conversion of the solid into the liquid phase, Figure 3. Equilibrium amounts versus temperature for sulfate roasting of spodumene using (a) confirmed by the sharp rise of the liquid phase with increasing temperature until around its melting Na2SO4, (b) K2SO4, (c) H2SO4, (d) SO3(g), (e) Fe2(SO4)3 and (f) Al2(SO4)3 (data from HSC Chemistry 5.1 point (462 ◦ C), where there is a total transformation into the liquid phase (Figure 4). software). Equilibrium amount (kmol) 2.0 1.5 H2O H2O(g) LiOH(l) 1.0 LiOH SiO2 Ca3Si2O7 0.5 Al2SiO5 Ca2Al2SiO7 N2(g) LiAlSi2O6(B) 0.0 0 200 400 600 800 1000 1200 Temperature (°C) Figure 4. Equilibrium amounts versus temperature for alkaline roasting of spodumene using CaOCaO Figure 4. Equilibrium amounts versus temperature for alkaline roasting of spodumene using (data(data fromfrom HSCHSC Chemistry 5.1 software). Chemistry 5.1 software). Figure 5a–c shows the modelling of chlorination roasting using CaCl2 , Cl2 and KCl, performed Figure 5a–c shows the modelling of chlorination roasting using CaCl2, Cl2 and KCl, performed experimentally by several authors [41,43,44,46]. From Figure 2, it is observed that the reactions with experimentally by several authors [41,43,44,46]. From Figure 2, it is observed that the reactions with CaCl2 and Cl2 are favored at a point or in the entire temperature range, however, it is not feasible with CaCl2 and Cl2 are favored at a point or in the entire temperature range, however, it is not feasible with KCl. This infeasibility is confirmed in Figure 5a where an appreciable mole of spodumene is observed KCl. This infeasibility is confirmed in Figure 5a where an appreciable mole of spodumene is observed in the equilibrium mixture. There is an onset production of solid LiCl which is converted into the liquid phase as soon as it is produced (Figure 5b,c). At ~610 °C (the melting point of lithium chloride) lithium chloride in the medium is predominantly in the liquid phase. A high volatilization phase (Figure 7) . On the other hand, the predicted reversal of the process at higher temperatures, signified by the rise of spodumene in their model with increasing temperature, was not observed in this study. The disparity may be attributed to the absence of liquid lithium fluoride in their model. Solid lithium fluoride begins to form but it melts and its amount decreases due to the simultaneous Metals 2020, 10, 1312 13 of 17one formation of the liquid phase with increasing temperature. The liquid phase becomes the stable at higher temperatures and its absence from the HSC equilibrium calculation leads to some errors in the result. There is a leveling of the liquid lithium Fluoride production at around 845 °C (the melting in the equilibrium mixture. There is an onset production of solid LiCl which is converted into the liquid point of LiF) due to the transformation of all of the solid phase into liquid. Their maximum extraction phase as soon as it is produced (Figure 5b,c). At ~610 ◦ C (the melting point of lithium chloride) lithium (~90%) occurred at 600 °C, which is just around what is predicted in this study. Gaseous lithium chloride in the medium is predominantly in the liquid phase. A high volatilization temperature is fluoride was not observed within this temperature range, but it is expected to appear around its expected due to the high vapor pressure of LiCl. Barbosa et al.  observed the gaseous phase at boiling point (1676 °C) and beyond. ~1000 ◦ C, however, it was not the case in the chlorination processes that were modelled. Equilibrium amount (kmol) 2.0 Equilibrium amount (kmol) 2.0 SiO2 Cl2(g) 1.5 SiO2(Q) 1.5 CaCl2 LiCl(l) 1.0 LiCl 0.5 LiCl(l) 1.0 LiAlSi2O6(B) Al2O3 CaAl2SiO6 0.5 LiCl O2(g) N2(g) 0.0 0 N2(g) 200 400 600 800 1000 0.0 1200 0 200 400 600 800 1000 1200 Temperature (°C) Temperature (°C) Metals 2020, 10, x FOR PEER REVIEW 14 of 18 (a) (b) Equilibrium amount (kmol) 0.9 KCl LiAlSi2O6(B) 0.8 0.7 0.6 LiCl 0.5 0.4 0.3 KAlSi2O6 KAlSiO4 0.2 0.1 KAlSi3O8 N2(g) SiO2 LiCl(g) 0.0 0 200 400 600 800 1000 1200 Temperature (°C) (c) Figure 5. Equilibrium amounts versus temperaturefor forchlorination chlorinationofofspodumene spodumeneusing using (a) (a) CaCl22,, (b) Figure 5. Equilibrium amounts versus temperature Cl 2 and (c) KCl (data from HSC Chemistry 5.1 software). (b) 2 and (c) KCl (data Carbonizing roasting of spodumene using Na2 CO3 as seen earlier in in Equations (12) and (13) Equilibrium amount (kmol) Equilibrium amount (kmol) 1.0 SiO2 1.0 can may yield either Li2 O or Li2 CO3 .The Li2 O that is produced produce SiO2 be made to go into leaching to CO2(g) Na2SiO3 0.9 Na2SiO3 Na2CO3 the reaction is not spontaneous LiOH but the prediction from the HSC software indicates0.9that except 0.8 0.8 for the production of Li2 CO3 (Figure 2). The infeasibility of Equation (12) is confirmed in Figure 6a, 0.7 0.7 where there is apparently, no leachable lithium product formed. The production of Li2 CO3 from this CO2(g) 0.6 0.6 Na2CO3 Al2SiO5 Al2SiO5 process0.5isLi2CO3 feasible below 700 ◦ C (Figure 2) which is confirmed in Figure 6bLi2O*SiO2 where Li2 CO3 is observed 0.5 ◦ 0.4 0.4 below this temperature. Around 300 C, the Li2 CO3 that was produced decomposes, forming carbon 0.3 0.3 dioxide, silicates, aluminates and aluminosilicates (Figure 6b). Thus, though there is feasibility until NaAlSiO4 Li2CO3 0.2 0.2 NaAlSiO4 LiAlSi2O6(B) Na2O*2SiO2 700 ◦ C,0.1it N2(g) is not recommended to operate up to this temperature due to the decomposition which occurs LiAlO2 N2(g) NaAlSi3O8 0.1 LiAlSiO4 NaAlSi3O8 Li2O NaAlSi2O6 NaAlSi2O6 *2Li2O*SiO2 Li2Al2O4 alongside the process. This confirms investigations by  0.0 that the ideal hydrothermal decomposition 0.0 0 200 400 600 800 1000 1200 C 0 200 400 600 800 1000 1200 (°C) ◦ C. It is mentioned that, the mixture Temperature (°C) temperature for the processTemperature as 90–225 of products from the decomposition process may be converted to sodic zeolite which when tapped increases the recovery (a) and the purity of lithium carbonate produced. 94% and 70% lithium recovery(b) were reached by working under high pressure and by adding sodium chloride, respectively, with this process [48,49]. using Figure 6. Equilibrium amounts versus temperature for carbonizing roasting of spodumene Na2CO3 by considering reactions reported in (a) Equation (12) and in (b) Equation (13), leading to the formation of Li2O and Li2CO3, respectively (data from HSC Chemistry 5.1 software). Equilibrium amount (kmol) 2.0 LiF LiF(l) 1.5 NaAlSiO4 0 200 400 600 800 1000 1200 Temperature (°C) (c) Metals 2020, 10, x FOR PEER REVIEW 14 of 18 Figure 5. Equilibrium amounts versus temperature for chlorination of spodumene using (a) CaCl2, (b) Metals 2020, 1312 14 of 17 Cl210, and (c) KCl (data from HSC Chemistry 5.1 software). Equilibrium amount (kmol) 0.9 KCl LiAlSi2O6(B) 0.8 Equilibrium amount (kmol) 1.0 SiO2 Equilibrium amount (kmol) 1.0 SiO2 0.7 Na2SiO3 0.9 0.8 0.5 0.7 0.4 0.6 Na2CO3 Li2CO3 Al2SiO5 Na2SiO3 LiCl 0.8 0.5 0.7 CO2(g) 0.9 Na2CO3 0.6 CO2(g) 0.6 0.3 0.5 Al2SiO5 Li2O*SiO2 KAlSi2O6 0.4 0.2 0.3 0.1 0.2 0.1 0.4 N2(g) 0 0 200 400 600 Li2O 400 600 800 1000 800 N2(g) 1000 NaAlSiO4 Na2O*2SiO2 1200 LiAlO2 LiAlSiO4 *2Li2O*SiO2 Li2Al2O4 0.1 Temperature (°C)NaAlSi3O8 NaAlSi3O8 200 SiO2 Li2CO3 LiCl(g) 0.2 LiAlSi2O6(B) NaAlSi2O6 0.0 KAlSi3O8 0.3 NaAlSiO4 0.0 N2(g) KAlSiO4 NaAlSi2O6 0.0 1200 0 200 400 600 (c) Temperature (°C) 800 1000 1200 C Temperature (°C) Figure 5. Equilibrium using (a) CaCl2, (b) (a) amounts versus temperature for chlorination of spodumene (b) Cl2 and (c) KCl (data from HSC Chemistry 5.1 software). Figure Equilibrium amounts versus temperature carbonizing roasting spodumene using Figure 6. 6. Equilibrium amounts versus temperature forfor carbonizing roasting of of spodumene using Na 2CO3 by considering reactions reported in (a) Equation (12) and in (b) Equation (13), leading to the Na2 CO3 by considering reactions reported in (a) Equation (12) and in (b) Equation (13), leading to the Equilibrium amount amount (kmol) 5.1 software). formation of(kmol) Li2O and Li2CO3, respectively (data fromEquilibrium HSC Chemistry formation of Li 1.0 1.0 Chemistry 5.1 software). 2 O and Li2 CO3 , respectively (data from HSC SiO2 SiO2 CO2(g) Na2SiO3 0.9 0.9 Na2CO3 Equilibrium amount (kmol) Na2SiO3 0.8 0.8 NaF is found favored throughout the Fluorination roasting2.0 of calcined spodumene using LiF LiF(l) 0.7 0.7 temperatures (Figure 2), which is confirmed by the formation of lithium fluoride in the solid or CO2(g) 0.6 0.6 liquid phase (Figure 7) . On the other hand, the predicted reversalLi2O*SiO2 of the process at higher Na2CO3 Li2CO3 Al2SiO5 Al2SiO5 0.5 0.5 1.5 temperatures, signified by the rise of spodumene in their model with increasing temperature, was not 0.4 0.4 NaAlSiO4 observed 0.3 to the absence of liquid lithium fluoride 0.3 in this study. The disparity may be attributed NaAlSiO4 Li2CO3 0.2 NaAlSiO4 in their 0.2model. Solid lithium fluoride begins to form but it melts and its amount decreases due LiAlSi2O6(B) 1.0 NaAlSi3O8 Na2O*2SiO2 LiAlO2 N2(g) N2(g) NaAlSi3O8 0.1 0.1 LiAlSiO4 to the simultaneous formation of the liquid phase with increasing temperature. The liquid phase NaAlSi3O8 Li2O NaAlSi2O6 NaAlSi2O6 *2Li2O*SiO2 Li2Al2O4 0.0 0.0 0 200 400HSC600 800 1000 1200 C 0 200 400 at higher 600 800 1000 1200 and its absence becomes the stable one temperatures from the equilibrium calculation Temperature (°C) Temperature (°C) 0.5 SiO2 leads to some errors in the result. There is a leveling of the liquid lithium Fluoride production at around 845 ◦ C (the melting of LiF) due to the transformation of all of the (a)point (b) solid phase into liquid. N2(g) LiAlSi2O6(B) NaF ◦ Their maximum extraction0.0(~90%) occurred at 600 C, which is just around what is predicted in this Figure 6. Equilibrium0 amounts for carbonizing roasting of spodumene using 200 versus 400 temperature 600 800 1000 1200 study. Gaseous lithium fluoride was not observed within this temperature range, but it is expected to Temperature (°C) Na2CO3 by considering reactions◦ reported in (a) Equation (12) and in (b) Equation (13), leading to the appear around its boiling point (1676 C) and beyond. formation of Li2O and Li2CO3, respectively (data from HSC Chemistry 5.1 software). Figure 7. Equilibrium amounts versus temperature for fluorination roasting of spodumene using NaF Equilibrium amount (kmol) (data from HSC Chemistry 5.1 software). 2.0 LiF LiF(l) 5. Conclusions 1.5 Besides the general review of the processes for spodumene treatment, an evaluation of the NaAlSiO4 chemical thermodynamics reveals that, sulfation, alkaline, fluorination, chlorination as well as 1.0 NaAlSi3O8 0.5 SiO2 N2(g) 0.0 0 LiAlSi2O6(B) NaF 200 400 600 800 1000 1200 Temperature (°C) Figure 7. Equilibrium amounts versus temperature for fluorination roasting of spodumene using NaF Figure 7. Equilibrium amounts versus temperature for fluorination roasting of spodumene using NaF (data from HSC Chemistry 5.1 software). (data from HSC Chemistry 5.1 software). 5. Conclusions 5. Conclusions Besides the general review of the processes for spodumene treatment, an evaluation of the chemical Besides the general of the processes for spodumene treatment, anasevaluation of the thermodynamics reveals that,review sulfation, alkaline, fluorination, chlorination as well carbonizing chemical thermodynamics reveals that, sulfation, alkaline, fluorination, chlorination as well to produce lithium carbonate were processes which had the required thermodynamic driving force as Metals 2020, 10, 1312 15 of 17 to move the reaction to the products for the reagents encountered in the literature. It is therefore not surprising sulfation (using sulfuric acid) and alkaline processes are considered as an industrial approach for lithium extraction. Looking at the mild nature of the reagents in the alkaline processes, it will be a real contender to the acidic process if the high energy requirement in the decomposition of limestone can be decreased by some means. Though roasting with lime is feasible even at lower temperatures, the decomposition of limestone is a precursor for the industrial production of lime which makes the overall process energy intensive. Future work must be focused on reducing the high heat needed for decomposing limestone to make the alkaline process economically viable. In the acid roasting process, SO3 and H2 O from the acid decomposition may drive the reaction to produce at a faster rate due to the higher diffusion rate of gases compared to liquids. In spite of the expected faster rate of reaction of these gases (SO3 and H2 O), little is known concerning their use for beneficiating lithium bearing minerals. It will be interesting if the behavior of these species as well as other gases are considered for processing lithium from ores. Sulfation as a method of spodumene beneficiation is mostly limited to sulfuric acid, with little focus on other sulfating reagents, but from the thermodynamics of this group of compounds it will also be interesting to pay attention to other members of this compound. There is considerable literature on the use of some alkali and alkaline earth metal sulfates as well as sulfates of ammonium for processing other lithium bearing minerals than spodumene. Even in those cases, there is minimal explanation of the chemical thermodynamics of the processes. Future work must therefore look at the use of other sulfating reagents for spodumene processing as well as their thermodynamics, both on spodumene and other lithium bearing minerals. Chlorination and fluorination have been found to be promising for lithium extraction. Few chlorination and fluorination agents are encountered in the literature for the process, despite their thermodynamic feasibility. More research should be pursued in search for new fluorination and chlorination agents and the processes should be optimized. The thermodynamics of the carbonizing process yielding lithium carbonate is very interesting; in particular its low operating temperature and the direct production of a considerably pure product. It is surprising that it has not attracted much attention. Further research must be pursued to optimize the process. From a thermodynamic point of view, temperatures below 300 ◦ C are predicted for the acid process and the feasible carbonizing process due to the acid and lithium carbonate decomposition. For the other processes discussed, temperatures less than 600 ◦ C are advised, except for fluorination, which works well a little above 600 ◦ C. Author Contributions: Conceptualization, A.C. and N.K. and software, A.Y.F. and N.K.; A.Y.F. writing—original draft preparation and writing—review and editing, A.C., N.K. and J.V.; Supervision, A.C. and N.K.; Funding acquisition, A.C. All authors have read and agreed to the published version of the manuscript. Funding: This work was supported by the French National Research Agency through the national program “Investissements d’avenir” with the reference ANR-10-LABX-21-RESSOURCES21. Conflicts of Interest: The authors declare no conflict of interest. References 1. 2. 3. 4. 5. Christmann, P.; Gloaguen, E.; Labbé, J.-F.; Melleton, J.; Piantone, P. Global Lithium Resources and Sustainability Issues. In Lithium Process Chemistry; Elsevier: Amsterdam, The Netherlands, 2015; pp. 1–40. ISBN 9780128014172. Meng, F.; McNeice, J.; Zadeh, S.S.; Ghahreman, A. Review of Lithium Production and Recovery from Minerals, Brines, and Lithium-Ion Batteries. Miner. Process. Extr. Metall. Rev. 2019, 1–19. [CrossRef] Pillot, C. The Rechargeable Battery Market and Main Trends 2015–2025. In Avicenne Energy, Proceedings of the 18th International Meeting on Lithium Batteries; Chicago, IL, USA, 19–24 June 2016, ENSAM: Paris, France, 2016. Salakjani, N.K.; Singh, P.; Nikoloski, A.N. Mineralogical transformations of spodumene concentrate from Greenbushes, Western Australia. Part 1: Conventional heating. Miner. Eng. 2016, 98, 71–79. [CrossRef] Salakjani, N.K.; Nikoloski, A.N.; Singh, P. Mineralogical transformations of spodumene concentrate from Greenbushes, Western Australia. Part 2: Microwave heating. Miner. Eng. 2017, 100, 191–199. [CrossRef] Metals 2020, 10, 1312 6. 7. 8. 9. 10. 11. 12. 13. 14. 15. 16. 17. 18. 19. 20. 21. 22. 23. 24. 25. 26. 27. 28. 29. 30. 31. 32. 16 of 17 Zelikman, A.N.; Belyaevskaya, L.V.; Samsonov, G.V.; Krein, O.E. Metallurgy of Rare Metals; Program for Scientific Translations: Jerusalem, Israel, 1966. Claffy, E.W. Composition, tenebrescence and luminescence of spodumene minerals. Am. Mineral. 1953, 38, 919–931. Gabriel, A.; Slavin, M.; Carl, H.F. Minor constituents in spodumene. Econ. Geol. 1942, 37, 116–125. [CrossRef] Salakjani, N.K.; Singh, P.; Nikoloski, A.N. Production of Lithium–A Literature Review Part 1: Pretreatment of Spodumene. Miner. Process. Extr. Metall. Rev. 2020, 41, 335–348. [CrossRef] Peltosaari, O.; Tanskanen, P.; Heikkinen, E.-P.; Fabritius, T. α→ γ→ β -phase transformation of spodumene with hybrid microwave and conventional furnaces. Miner. Eng. 2015, 82, 54–60. [CrossRef] Abdullah, A.A.; Oskierski, H.C.; Altarawneh, M.; Senanayake, G.; Lumpkin, G.; Dlugogorski, B.Z. Phase transformation mechanism of spodumene during its calcination. Miner. Eng. 2019, 140, 105883. [CrossRef] Fraas, F.; Ralston, O.C.; States., U.; Mines., B. Beneficiation of Spodumene by Decrepitation; U.S. Deptartment of the Interior; Bureau of Mines: Washington, WA, USA, 1937. Dessemond, C.; Lajoie-Leroux, F.; Soucy, G.; Laroche, N.; Magnan, J.-F. Spodumene: The Lithium Market, Resources and Processes. Minerals 2019, 9, 334. [CrossRef] White, G.D.; McVay, T.N. Some Aspects of the Recovery of Lithium from Spodumene; Oak Ridge National Laboratory: Oak Ridge, TN, USA, 1958. Guo, H.; Kuang, G.; Wang, H.; Yu, H.; Zhao, X. Investigation of Enhanced Leaching of Lithium from α-Spodumene Using Hydrofluoric and Sulfuric Acid. Minerals 2017, 7, 205. [CrossRef] Moore, R.L.; Mann, J.P.; Montoya, A.; Haynes, B.S. In situ synchrotron XRD analysis of the kinetics of spodumene phase transitions. Phys. Chem. Chem. Phys. 2018, 20, 10753–10761. [CrossRef] [PubMed] Dwyer, T.E. Recovery of Lithium from Spodumene Ores. U.S. Patent No. 2801153A, 30 July 1957. Gasalla, H.; Pereira, E. Activation-deactivation mechanisms in spodumene samples. Solid State Ion. 1990, 42, 1–6. [CrossRef] Salakjani, N.K.; Singh, P.; Nikoloski, A.N. Acid roasting of spodumene: Microwave vs. conventional heating. Miner. Eng. 2019, 138, 161–167. [CrossRef] Choubey, P.K.; Kim, M.; Srivastava, R.R.; Lee, J.; Lee, J.-Y. Advance review on the exploitation of the prominent energy-storage element: Lithium. Part I: From mineral and brine resources. Miner. Eng. 2016, 89, 119–137. [CrossRef] Meshram, P.; Pandey, B.D.; Mankhand, T.R. Extraction of lithium from primary and secondary sources by pre-treatment, leaching and separation: A comprehensive review. Hydrometallurgy 2014, 150, 192–208. [CrossRef] Yan, Q.; Li, X.; Wang, Z.; Wu, X.; Guo, H.; Hu, Q.; Peng, W.; Wang, J. Extraction of valuable metals from lepidolite. Hydrometallurgy 2012, 117–118, 116–118. [CrossRef] Luong, V.T.; Kang, D.J.; An, J.W.; Kim, M.J.; Tran, T. Factors affecting the extraction of lithium from lepidolite. Hydrometallurgy 2013, 134–135, 54–61. [CrossRef] Luong, V.T.; Kang, D.J.; An, J.W.; Dao, D.A.; Kim, M.J.; Tran, T. Iron sulphate roasting for extraction of lithium from lepidolite. Hydrometallurgy 2014, 141, 8–16. [CrossRef] Siame, E.; Pascoe, R.D. Extraction of lithium from micaceous waste from china clay production. Miner. Eng. 2011, 24, 1595–1602. [CrossRef] Sitando, O.; Crouse, P.L. Processing of a Zimbabwean petalite to obtain lithium carbonate. Int. J. Miner. Process. 2012, 102, 45–50. [CrossRef] Amer, A.M. The hydrometallurgical extraction of lithium from egyptian montmorillonite-type clay. JOM 2008, 60, 55–57. [CrossRef] Kuang, G.; Liu, Y.; Li, H.; Xing, S.; Li, F.; Guo, H. Extraction of lithium from β-spodumene using sodium sulfate solution. Hydrometallurgy 2018, 177, 49–56. [CrossRef] Lajoie-Leroux, F.; Dessemond, C.; Soucy, G.; Laroche, N.; Magnan, J.-F. Impact of the impurities on lithium extraction from β-spodumene in the sulfuric acid process. Miner. Eng. 2018, 129, 1–8. [CrossRef] Tian, Q.; Chen, B.; Chen, Y.; Ma, L.; Shi, X. Roasting and leaching behavior of spodumene in sulphuric acid process. Chin. J. Rare Met. 2011, 35, 118–123. [CrossRef] Ellestad, R.B.; Milne, L. Method of Extracting Lithium Values From Spodumene Ores. U.S. Patent No. 2,516,109, 25 July 1950. Maurice, A.; Macewan, J.U.; Olivier, C.A. Method of Producing Lithium Carbonate from Spodumene. U.S. Patent No. 3,017,243, 16 January 1962. Metals 2020, 10, 1312 33. 34. 35. 36. 37. 38. 39. 40. 41. 42. 43. 44. 45. 46. 47. 48. 49. 50. 51. 52. 53. 54. 55. 17 of 17 Jandová, J.; Dvořák, P.; Vu, H.N. Processing of zinnwaldite waste to obtain Li2CO3. Hydrometallurgy 2010, 103, 12–18. [CrossRef] Mcintosh, N. Production of Lithium Compounds. U.S. Patent No. 2,413,644, 31 December 1946. Jandová, J.; Vu, H.N.; Kondas, J.; Dvořák, P. Lithium recovery from wastes after mining of Sn-W ore. In Proceedings of the European Metallurgical Conference, EMC 2007, Düsseldorf, Germany, 11–14 June 2007; pp. 667–677. Jandova, J.; Vu, H.N. Processing of zinnwaldite wastes to obtain lithium and rubidium compounds. In Proceedings of the 2008 Global Symposium on Recycling, Waste Treatment and Clean Technology, REWAS 2008, Cancun, Mexico, 12–15 October, 2008. Jandová, J.; Vu, H.N.; Beloková, T.; DvořÁk, P.; Kondás, J. Obtaining Li2CO3 from Zinnwaldite wastes. Ceram. Silik. 2009, 53, 108–112. Kanari, N.; Allain, E.; Joussemet, R.; Mochón, J.; Ruiz-Bustinza, I.; Gaballah, I. An overview study of chlorination reactions applied to the primary extraction and recycling of metals and to the synthesis of new reagents. Thermochim. Acta 2009, 495, 42–50. [CrossRef] Kanari, N.; Mishra, D.; Mochón, J.; Verdeja, L.F.; Diot, F.; Allain, E. Some kinetics aspects of chlorine-solids reactions. Rev. Metal. 2010, 46, 22–36. [CrossRef] Gaballah, J.; Kanari, N.; Djona, M. Use of chlorine for mineral processing, metal extraction and recycling via synthesis of new reagent. Chloride Metall. 2002, 1, 203–225. Peterson, J.A.; Glioss, G.H. Lithium Values Recovery Process. U.S. Patent No. 2,893,828, 7 July 1959. Yan, Q.; Li, X.; Wang, Z.; Wang, J.; Guo, H.; Hu, Q.; Peng, W.; Wu, X. Extraction of lithium from lepidolite using chlorination roasting–water leaching process. Trans. Nonferrous Met. Soc. China 2012, 22, 1753–1759. [CrossRef] Barbosa, L.I.; Valente, G.; Orosco, R.P.; González, J.A. Lithium extraction from β-spodumene through chlorination with chlorine gas. Miner. Eng. 2014, 56, 29–34. [CrossRef] Barbosa, L.I.; González, J.A.; del Carmen Ruiz, M. Extraction of lithium from β-spodumene using chlorination roasting with calcium chloride. Thermochim. Acta 2015, 605, 63–67. [CrossRef] Dang, H.; Li, N.; Chang, Z.; Wang, B.; Zhan, Y.; Wu, X.; Liu, W.; Ali, S.; Li, H.; Guo, J.; et al. Lithium leaching via calcium chloride roasting from simulated pyrometallurgical slag of spent lithium ion battery. Sep. Purif. Technol. 2020, 233, 116025. [CrossRef] Erasmus, H.D. Method of Treating Lithiferous Ores to Recover Lithium as Lithium Chloride. U.S. Patent No. 2,561,439, 24 July 1951. Maurice, A.; Olivier, C.A. Carbonatizing Roast of Lithium Bearing Ores. U.S. Patent No. 3,380,802, 30 April 1968. Chen, Y.; Tian, Q.; Chen, B.; Shi, X.; Liao, T. Preparation of lithium carbonate from spodumene by a sodium carbonate autoclave process. Hydrometallurgy 2011, 109, 43–46. [CrossRef] Dos Santos, L.L.; do Nascimento, R.M.; Pergher, S.B.C. Beta-spodumene: Na2 CO3 : NaCl system calcination: A kinetic study of the conversion to lithium salt. Chem. Eng. Res. Des. 2019, 147, 338–345. [CrossRef] Rosales, G.D.; Resentera, A.C.J.; Gonzalez, J.A.; Wuilloud, R.G.; Rodriguez, M.H. Efficient extraction of lithium from β-spodumene by direct roasting with NaF and leaching. Chem. Eng. Res. Des. 2019, 150, 320–326. [CrossRef] Rosales, G.D.; Ruiz, M.D.C.; Rodriguez, M.H. Novel process for the extraction of lithium from β-spodumene by leaching with HF. Hydrometallurgy 2014, 147–148, 1–6. [CrossRef] Robinson, G.P. Recovery of Lithium from Ore. U.S. Patent No. 2,983,576, 9 May 1961. Hayes, E.T.; Williams, F.P.; Sternberg, W. Production of Lithium Chloride from Spodumene. U.S. Patent No. 2,533,246, 12 December 1950. Sharratt, H.J. The Extraction of Lithium from Spodumene. Master’s Thesis, McGill University, Montreal, QC, Canada, 1955. Salakjani, N.K.; Singh, P.; Nikoloski, A.N. Production of Lithium–A Literature Review. Part 2. Extraction from Spodumene. Miner. Process. Extr. Metall. Rev. 2019, 1–16. [CrossRef] © 2020 by the authors. Licensee MDPI, Basel, Switzerland. This article is an open access article distributed under the terms and conditions of the Creative Commons Attribution (CC BY) license (http://creativecommons.org/licenses/by/4.0/).